 
data_metahew 
 
_audit_creation_method            SHELXL-97 
_chemical_name_systematic 
; 
 ? 
; 
_chemical_name_common             ? 
_chemical_melting_point           ? 
_chemical_formula_moiety          ? 
_chemical_formula_sum 
 'H6 Ca O19 V6' 
_chemical_formula_weight          655.77 
 
loop_ 
 _atom_type_symbol 
 _atom_type_description 
 _atom_type_scat_dispersion_real 
 _atom_type_scat_dispersion_imag 
 _atom_type_scat_source 
 'O'  'O'   0.0106   0.0060 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'H'  'H'   0.0000   0.0000 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Ca'  'Ca'   0.2262   0.3064 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'V'  'V'   0.3005   0.5294 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 
_symmetry_cell_setting            ? 
_symmetry_space_group_name_H-M    ? 
 
loop_ 
 _symmetry_equiv_pos_as_xyz 
 'x, y, z' 
 '-x, y, -z' 
 'x, y+1/2, z+1/2' 
 '-x, y+1/2, -z+1/2' 
 '-x, -y, -z' 
 'x, -y, z' 
 '-x, -y+1/2, -z+1/2' 
 'x, -y+1/2, z+1/2' 
 
_cell_length_a                    12.208(5) 
_cell_length_b                    3.6011(15) 
_cell_length_c                    18.358(7) 
_cell_angle_alpha                 90.00 
_cell_angle_beta                  118.538(8) 
_cell_angle_gamma                 90.00 
_cell_volume                      709.0(5) 
_cell_formula_units_Z             2 
_cell_measurement_temperature     293(2) 
_cell_measurement_reflns_used     ? 
_cell_measurement_theta_min       ? 
_cell_measurement_theta_max       ? 
 
_exptl_crystal_description        ? 
_exptl_crystal_colour             ? 
_exptl_crystal_size_max           ? 
_exptl_crystal_size_mid           ? 
_exptl_crystal_size_min           ? 
_exptl_crystal_density_meas       ? 
_exptl_crystal_density_diffrn     3.072 
_exptl_crystal_density_method     'not measured' 
_exptl_crystal_F_000              632 
_exptl_absorpt_coefficient_mu     4.263 
_exptl_absorpt_correction_type    ? 
_exptl_absorpt_correction_T_min   ? 
_exptl_absorpt_correction_T_max   ? 
_exptl_absorpt_process_details    ? 
 
_exptl_special_details 
; 
 ? 
; 
 
_diffrn_ambient_temperature       293(2) 
_diffrn_radiation_wavelength      0.71073 
_diffrn_radiation_type            MoK\a 
_diffrn_radiation_source          'fine-focus sealed tube' 
_diffrn_radiation_monochromator   graphite 
_diffrn_measurement_device_type   ? 
_diffrn_measurement_method        ? 
_diffrn_detector_area_resol_mean  ? 
_diffrn_standards_number          ? 
_diffrn_standards_interval_count  ? 
_diffrn_standards_interval_time   ? 
_diffrn_standards_decay_%         ? 
_diffrn_reflns_number             4091 
_diffrn_reflns_av_R_equivalents   0.0244 
_diffrn_reflns_av_sigmaI/netI     0.0215 
_diffrn_reflns_limit_h_min        -17 
_diffrn_reflns_limit_h_max        17 
_diffrn_reflns_limit_k_min        -5 
_diffrn_reflns_limit_k_max        5 
_diffrn_reflns_limit_l_min        -25 
_diffrn_reflns_limit_l_max        25 
_diffrn_reflns_theta_min          1.90 
_diffrn_reflns_theta_max          30.10 
_reflns_number_total              1182 
_reflns_number_gt                 1047 
_reflns_threshold_expression      >2sigma(I) 
 
_computing_data_collection        ? 
_computing_cell_refinement        ? 
_computing_data_reduction         ? 
_computing_structure_solution     'SHELXS-97 (Sheldrick, 1990)' 
_computing_structure_refinement   'SHELXL-97 (Sheldrick, 1997)' 
_computing_molecular_graphics     ? 
_computing_publication_material   ? 
 
_refine_special_details 
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
; 
 
_refine_ls_structure_factor_coef  Fsqd  
_refine_ls_matrix_type            full 
_refine_ls_weighting_scheme       calc  
_refine_ls_weighting_details 
 'calc w=1/[σ²(Fo²)+(0.0242P)²+2.4445P] where P=(Fo²+2Fc²)/3' 
_atom_sites_solution_primary      direct 
_atom_sites_solution_secondary    difmap 
_atom_sites_solution_hydrogens    geom 
_refine_ls_hydrogen_treatment     mixed 
_refine_ls_extinction_method      SHELXL 
_refine_ls_extinction_coef        0.0006(3) 
_refine_ls_extinction_expression 
 'Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^' 
_refine_ls_number_reflns          1182 
_refine_ls_number_parameters      90 
_refine_ls_number_restraints      0 
_refine_ls_R_factor_all           0.0301 
_refine_ls_R_factor_gt            0.0244 
_refine_ls_wR_factor_ref          0.0667 
_refine_ls_wR_factor_gt           0.0649 
_refine_ls_goodness_of_fit_ref    1.156 
_refine_ls_restrained_S_all       1.156 
_refine_ls_shift/su_max           0.000 
_refine_ls_shift/su_mean          0.000 
 
loop_ 
 _atom_site_label 
 _atom_site_type_symbol 
 _atom_site_fract_x 
 _atom_site_fract_y 
 _atom_site_fract_z 
 _atom_site_U_iso_or_equiv 
 _atom_site_adp_type 
 _atom_site_occupancy 
 _atom_site_symmetry_multiplicity 
 _atom_site_calc_flag 
 _atom_site_refinement_flags 
 _atom_site_disorder_assembly 
 _atom_site_disorder_group 
Ca1 Ca 0.5139(15) 0.0000 0.0073(13) 0.0187(19) Uani 0.25 2 d SP . . 
Ca2 Ca 0.1056(3) 0.5000 0.03623(19) 0.0283(7) Uani 0.25 2 d SP . . 
V1 V 0.02216(5) 0.5000 0.19006(3) 0.01103(13) Uani 1 2 d S . . 
V2 V 0.39980(5) 0.0000 0.16948(3) 0.01001(13) Uani 1 2 d S . . 
V3 V 0.31311(5) 0.5000 0.27707(3) 0.01379(14) Uani 1 2 d S . . 
O1 O -0.0934(2) 0.5000 0.09774(16) 0.0224(5) Uani 1 2 d S . . 
O2 O 0.2711(2) 0.0000 0.08403(16) 0.0218(5) Uani 1 2 d S . . 
O3 O 0.2582(2) 0.5000 0.34076(16) 0.0216(5) Uani 1 2 d S . . 
O4 O 0.1530(2) 0.5000 0.17620(14) 0.0141(4) Uani 1 2 d S . . 
O5 O 0.5113(2) 0.0000 0.13539(14) 0.0140(4) Uani 1 2 d S . . 
O6 O 0.32830(19) 0.0000 0.25564(14) 0.0131(4) Uani 1 2 d S . . 
O7 O 0.0353(2) 0.0000 0.22528(15) 0.0150(4) Uani 1 2 d S . . 
O8 O 0.4160(2) 0.5000 0.20396(14) 0.0128(4) Uani 1 2 d S . . 
OW1 O 0.6319(3) 0.5000 0.01589(19) 0.0365(7) Uani 1 2 d S . . 
OW2 O 0.0110(10) 0.044(3) 0.0089(7) 0.032(2) Uiso 0.25 1 d P . . 
 
 
_geom_special_details 
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
; 
 
loop_ 
 _geom_bond_atom_site_label_1 
 _geom_bond_atom_site_label_2 
 _geom_bond_distance 
 _geom_bond_site_symmetry_2 
 _geom_bond_publ_flag 
Ca1 Ca1 0.32(3) 5_655 ? 
Ca1 OW1 2.264(14) . ? 
Ca1 OW1 2.264(14) 1_545 ? 
Ca1 O5 2.37(3) . ? 
Ca1 OW1 2.422(14) 5_655 ? 
Ca1 OW1 2.422(14) 5_665 ? 
Ca1 O5 2.49(3) 5_655 ? 
Ca1 O3 2.847(13) 7_655 ? 
Ca1 O3 3.158(13) 3_544 ? 
Ca1 V3 3.484(19) 7_655 ? 
Ca1 Ca1 3.6011(15) 1_565 ? 
Ca1 Ca1 3.6011(15) 1_545 ? 
Ca1 Ca1 3.615(3) 5_645 ? 
Ca1 Ca1 3.615(3) 5_665 ? 
Ca1 V3 3.738(18) 3_544 ? 
Ca1 V2 3.84(3) . ? 
Ca1 V2 3.86(3) 5_655 ? 
Ca2 OW2 1.932(12) . ? 
Ca2 OW2 1.932(12) 6_565 ? 
Ca2 OW2 2.070(10) 2 ? 
Ca2 OW2 2.070(10) 5_565 ? 
Ca2 OW2 2.205(10) 6 ? 
Ca2 OW2 2.205(10) 1_565 ? 
Ca2 Ca2 2.267(7) 5_565 ? 
Ca2 OW2 2.327(12) 5 ? 
Ca2 OW2 2.327(12) 2_565 ? 
Ca2 O4 2.349(4) . ? 
Ca2 O1 2.392(4) 5_565 ? 
Ca2 O2 2.530(3) 1_565 ? 
Ca2 O2 2.530(3) . ? 
Ca2 O1 3.130(4) . ? 
Ca2 V1 3.429(4) . ? 
Ca2 Ca2 3.6011(15) 1_565 ? 
Ca2 Ca2 3.6011(15) 1_545 ? 
Ca2 V1 3.674(3) 5_565 ? 
Ca2 V2 3.706(3) 1_565 ? 
Ca2 V2 3.706(3) . ? 
V1 O1 1.606(3) . ? 
V1 O4 1.733(2) . ? 
V1 O7 1.8938(10) 1_565 ? 
V1 O7 1.8938(10) . ? 
V1 O7 1.987(2) 7 ? 
V1 O3 2.888(3) . ? 
V1 V1 3.0846(12) 7_565 ? 
V1 V1 3.0846(12) 7 ? 
V1 V3 3.1219(15) . ? 
V1 V1 3.6011(15) 1_565 ? 
V1 V1 3.6011(15) 1_545 ? 
V1 Ca2 3.674(3) 5_565 ? 
V2 O2 1.604(2) . ? 
V2 O5 1.749(2) . ? 
V2 O8 1.8874(10) . ? 
V2 O8 1.8874(10) 1_545 ? 
V2 O6 2.141(2) . ? 
V2 O8 2.337(2) 7_655 ? 
V2 V3 3.1561(16) 7_655 ? 
V2 V3 3.2033(10) . ? 
V2 V3 3.2033(10) 1_545 ? 
V2 V2 3.3253(12) 7_655 ? 
V2 V2 3.3253(12) 7_645 ? 
V2 V2 3.6011(15) 1_545 ? 
V2 V2 3.6011(15) 1_565 ? 
V2 Ca2 3.706(3) 1_545 ? 
V3 O3 1.602(2) . ? 
V3 O6 1.8711(9) 1_565 ? 
V3 O6 1.8711(9) . ? 
V3 O4 1.947(2) . ? 
V3 O5 1.971(2) 7_655 ? 
V3 O8 2.234(2) . ? 
V3 V2 3.1561(16) 7_655 ? 
V3 V2 3.2033(10) 1_565 ? 
V3 Ca1 3.484(19) 7_655 ? 
V3 V3 3.6011(15) 1_565 ? 
V3 V3 3.6011(15) 1_545 ? 
V3 Ca1 3.738(18) 3 ? 
O1 Ca2 2.392(4) 5_565 ? 
O2 Ca2 2.530(3) 1_545 ? 
O3 Ca1 2.847(13) 7_655 ? 
O3 Ca1 3.158(13) 3 ? 
O5 V3 1.971(2) 7_655 ? 
O5 Ca1 2.49(3) 5_655 ? 
O6 V3 1.8711(9) 1_545 ? 
O7 V1 1.8938(10) 1_545 ? 
O7 V1 1.987(2) 7 ? 
O8 V2 1.8874(10) 1_565 ? 
O8 V2 2.337(2) 7_655 ? 
OW1 Ca1 2.264(14) 1_565 ? 
OW1 Ca1 2.422(14) 5_655 ? 
OW1 Ca1 2.422(14) 5_665 ? 
OW2 OW2 0.31(2) 2 ? 
OW2 OW2 0.31(2) 6 ? 
OW2 OW2 0.44(2) 5 ? 
OW2 Ca2 2.070(10) 5_565 ? 
OW2 Ca2 2.205(10) 1_545 ? 
OW2 Ca2 2.327(12) 5 ? 
 
loop_ 
 _geom_angle_atom_site_label_1 
 _geom_angle_atom_site_label_2 
 _geom_angle_atom_site_label_3 
 _geom_angle 
 _geom_angle_site_symmetry_1 
 _geom_angle_site_symmetry_3 
 _geom_angle_publ_flag 
Ca1 Ca1 OW1 117(5) 5_655 . ? 
Ca1 Ca1 OW1 117(5) 5_655 1_545 ? 
OW1 Ca1 OW1 105.3(9) . 1_545 ? 
Ca1 Ca1 O5 109(10) 5_655 . ? 
OW1 Ca1 O5 104.0(6) . . ? 
OW1 Ca1 O5 104.0(6) 1_545 . ? 
Ca1 Ca1 OW1 57(5) 5_655 5_655 ? 
OW1 Ca1 OW1 173.3(6) . 5_655 ? 
OW1 Ca1 OW1 79.11(13) 1_545 5_655 ? 
O5 Ca1 OW1 79.5(8) . 5_655 ? 
Ca1 Ca1 OW1 57(5) 5_655 5_665 ? 
OW1 Ca1 OW1 79.11(13) . 5_665 ? 
OW1 Ca1 OW1 173.3(6) 1_545 5_665 ? 
O5 Ca1 OW1 79.5(8) . 5_665 ? 
OW1 Ca1 OW1 96.0(7) 5_655 5_665 ? 
Ca1 Ca1 O5 64(10) 5_655 5_655 ? 
OW1 Ca1 O5 80.1(8) . 5_655 ? 
OW1 Ca1 O5 80.1(8) 1_545 5_655 ? 
O5 Ca1 O5 173.1(8) . 5_655 ? 
OW1 Ca1 O5 96.0(5) 5_655 5_655 ? 
OW1 Ca1 O5 96.0(5) 5_665 5_655 ? 
Ca1 Ca1 O3 169(10) 5_655 7_655 ? 
OW1 Ca1 O3 68.9(3) . 7_655 ? 
OW1 Ca1 O3 68.9(3) 1_545 7_655 ? 
O5 Ca1 O3 59.8(4) . 7_655 ? 
OW1 Ca1 O3 117.7(6) 5_655 7_655 ? 
OW1 Ca1 O3 117.7(6) 5_665 7_655 ? 
O5 Ca1 O3 127.1(10) 5_655 7_655 ? 
Ca1 Ca1 O3 10(10) 5_655 3_544 ? 
OW1 Ca1 O3 111.7(6) . 3_544 ? 
OW1 Ca1 O3 111.7(6) 1_545 3_544 ? 
O5 Ca1 O3 119.1(9) . 3_544 ? 
OW1 Ca1 O3 61.7(3) 5_655 3_544 ? 
OW1 Ca1 O3 61.7(3) 5_665 3_544 ? 
O5 Ca1 O3 54.0(3) 5_655 3_544 ? 
O3 Ca1 O3 178.9(11) 7_655 3_544 ? 
Ca1 Ca1 V3 142(10) 5_655 7_655 ? 
OW1 Ca1 V3 84.3(4) . 7_655 ? 
OW1 Ca1 V3 84.3(4) 1_545 7_655 ? 
O5 Ca1 V3 32.8(2) . 7_655 ? 
OW1 Ca1 V3 101.3(7) 5_655 7_655 ? 
OW1 Ca1 V3 101.3(7) 5_665 7_655 ? 
O5 Ca1 V3 154.1(8) 5_655 7_655 ? 
O3 Ca1 V3 27.0(2) 7_655 7_655 ? 
O3 Ca1 V3 151.9(9) 3_544 7_655 ? 
Ca1 Ca1 Ca1 90.000(4) 5_655 1_565 ? 
OW1 Ca1 Ca1 37.3(5) . 1_565 ? 
OW1 Ca1 Ca1 142.7(5) 1_545 1_565 ? 
O5 Ca1 Ca1 90.0 . 1_565 ? 
OW1 Ca1 Ca1 138.0(4) 5_655 1_565 ? 
OW1 Ca1 Ca1 42.0(4) 5_665 1_565 ? 
O5 Ca1 Ca1 90.0 5_655 1_565 ? 
O3 Ca1 Ca1 90.0 7_655 1_565 ? 
O3 Ca1 Ca1 90.0 3_544 1_565 ? 
V3 Ca1 Ca1 90.0 7_655 1_565 ? 
Ca1 Ca1 Ca1 90.000(5) 5_655 1_545 ? 
OW1 Ca1 Ca1 142.7(5) . 1_545 ? 
OW1 Ca1 Ca1 37.3(5) 1_545 1_545 ? 
O5 Ca1 Ca1 90.0 . 1_545 ? 
OW1 Ca1 Ca1 42.0(4) 5_655 1_545 ? 
OW1 Ca1 Ca1 138.0(4) 5_665 1_545 ? 
O5 Ca1 Ca1 90.0 5_655 1_545 ? 
O3 Ca1 Ca1 90.0 7_655 1_545 ? 
O3 Ca1 Ca1 90.0 3_544 1_545 ? 
V3 Ca1 Ca1 90.0 7_655 1_545 ? 
Ca1 Ca1 Ca1 180.000(1) 1_565 1_545 ? 
Ca1 Ca1 Ca1 85.0(4) 5_655 5_645 ? 
OW1 Ca1 Ca1 146.2(13) . 5_645 ? 
OW1 Ca1 Ca1 41.1(3) 1_545 5_645 ? 
O5 Ca1 Ca1 91.6(9) . 5_645 ? 
OW1 Ca1 Ca1 38.0(3) 5_655 5_645 ? 
OW1 Ca1 Ca1 133.8(10) 5_665 5_645 ? 
O5 Ca1 Ca1 87.8(8) 5_655 5_645 ? 
O3 Ca1 Ca1 94.9(4) 7_655 5_645 ? 
O3 Ca1 Ca1 85.1(4) 3_544 5_645 ? 
V3 Ca1 Ca1 94.0(6) 7_655 5_645 ? 
Ca1 Ca1 Ca1 175.0(4) 1_565 5_645 ? 
Ca1 Ca1 Ca1 5.0(4) 1_545 5_645 ? 
Ca1 Ca1 Ca1 85.0(4) 5_655 5_665 ? 
OW1 Ca1 Ca1 41.1(3) . 5_665 ? 
OW1 Ca1 Ca1 146.2(13) 1_545 5_665 ? 
O5 Ca1 Ca1 91.6(9) . 5_665 ? 
OW1 Ca1 Ca1 133.8(10) 5_655 5_665 ? 
OW1 Ca1 Ca1 38.0(3) 5_665 5_665 ? 
O5 Ca1 Ca1 87.8(8) 5_655 5_665 ? 
O3 Ca1 Ca1 94.9(4) 7_655 5_665 ? 
O3 Ca1 Ca1 85.1(4) 3_544 5_665 ? 
V3 Ca1 Ca1 94.0(6) 7_655 5_665 ? 
Ca1 Ca1 Ca1 5.0(4) 1_565 5_665 ? 
Ca1 Ca1 Ca1 175.0(4) 1_545 5_665 ? 
Ca1 Ca1 Ca1 170.0(8) 5_645 5_665 ? 
Ca1 Ca1 V3 35(10) 5_655 3_544 ? 
OW1 Ca1 V3 97.5(7) . 3_544 ? 
OW1 Ca1 V3 97.5(7) 1_545 3_544 ? 
O5 Ca1 V3 144.2(8) . 3_544 ? 
OW1 Ca1 V3 76.8(3) 5_655 3_544 ? 
OW1 Ca1 V3 76.8(3) 5_665 3_544 ? 
O5 Ca1 V3 28.93(17) 5_655 3_544 ? 
O3 Ca1 V3 156.0(10) 7_655 3_544 ? 
O3 Ca1 V3 25.09(17) 3_544 3_544 ? 
V3 Ca1 V3 177.0(8) 7_655 3_544 ? 
Ca1 Ca1 V3 90.0 1_565 3_544 ? 
Ca1 Ca1 V3 90.0 1_545 3_544 ? 
Ca1 Ca1 V3 85.9(6) 5_645 3_544 ? 
Ca1 Ca1 V3 85.9(6) 5_665 3_544 ? 
Ca1 Ca1 V2 91(10) 5_655 . ? 
OW1 Ca1 V2 113.6(7) . . ? 
OW1 Ca1 V2 113.6(7) 1_545 . ? 
O5 Ca1 V2 17.9(3) . . ? 
OW1 Ca1 V2 68.2(6) 5_655 . ? 
OW1 Ca1 V2 68.2(6) 5_665 . ? 
O5 Ca1 V2 155.2(6) 5_655 . ? 
O3 Ca1 V2 77.7(6) 7_655 . ? 
O3 Ca1 V2 101.2(6) 3_544 . ? 
V3 Ca1 V2 50.7(4) 7_655 . ? 
Ca1 Ca1 V2 90.0 1_565 . ? 
Ca1 Ca1 V2 90.0 1_545 . ? 
Ca1 Ca1 V2 90.1(9) 5_645 . ? 
Ca1 Ca1 V2 90.1(9) 5_665 . ? 
V3 Ca1 V2 126.3(5) 3_544 . ? 
Ca1 Ca1 V2 84(10) 5_655 5_655 ? 
OW1 Ca1 V2 68.8(7) . 5_655 ? 
OW1 Ca1 V2 68.8(7) 1_545 5_655 ? 
O5 Ca1 V2 166.8(6) . 5_655 ? 
OW1 Ca1 V2 109.0(6) 5_655 5_655 ? 
OW1 Ca1 V2 109.0(6) 5_665 5_655 ? 
O5 Ca1 V2 20.1(3) 5_655 5_655 ? 
O3 Ca1 V2 107.0(7) 7_655 5_655 ? 
O3 Ca1 V2 74.1(5) 3_544 5_655 ? 
V3 Ca1 V2 134.0(6) 7_655 5_655 ? 
Ca1 Ca1 V2 90.000(1) 1_565 5_655 ? 
Ca1 Ca1 V2 90.0 1_545 5_655 ? 
Ca1 Ca1 V2 89.5(9) 5_645 5_655 ? 
Ca1 Ca1 V2 89.5(9) 5_665 5_655 ? 
V3 Ca1 V2 49.0(3) 3_544 5_655 ? 
V2 Ca1 V2 175.3(4) . 5_655 ? 
OW2 Ca2 OW2 116.6(6) . 6_565 ? 
OW2 Ca2 OW2 7.9(6) . 2 ? 
OW2 Ca2 OW2 111.1(4) 6_565 2 ? 
OW2 Ca2 OW2 111.1(4) . 5_565 ? 
OW2 Ca2 OW2 7.9(6) 6_565 5_565 ? 
OW2 Ca2 OW2 105.1(7) 2 5_565 ? 
OW2 Ca2 OW2 4.3(3) . 6 ? 
OW2 Ca2 OW2 120.9(6) 6_565 6 ? 
OW2 Ca2 OW2 11.2(6) 2 6 ? 
OW2 Ca2 OW2 115.38(16) 5_565 6 ? 
OW2 Ca2 OW2 120.9(6) . 1_565 ? 
OW2 Ca2 OW2 4.3(3) 6_565 1_565 ? 
OW2 Ca2 OW2 115.38(16) 2 1_565 ? 
OW2 Ca2 OW2 11.2(6) 5_565 1_565 ? 
OW2 Ca2 OW2 125.2(7) 6 1_565 ? 
OW2 Ca2 Ca2 58.4(3) . 5_565 ? 
OW2 Ca2 Ca2 58.4(3) 6_565 5_565 ? 
OW2 Ca2 Ca2 52.7(3) 2 5_565 ? 
OW2 Ca2 Ca2 52.7(3) 5_565 5_565 ? 
OW2 Ca2 Ca2 62.7(3) 6 5_565 ? 
OW2 Ca2 Ca2 62.7(3) 1_565 5_565 ? 
OW2 Ca2 OW2 5.2(6) . 5 ? 
OW2 Ca2 OW2 115.79(17) 6_565 5 ? 
OW2 Ca2 OW2 4.7(3) 2 5 ? 
OW2 Ca2 OW2 109.8(5) 5_565 5 ? 
OW2 Ca2 OW2 7.1(5) 6 5 ? 
OW2 Ca2 OW2 120.1(3) 1_565 5 ? 
Ca2 Ca2 OW2 57.4(3) 5_565 5 ? 
OW2 Ca2 OW2 115.79(17) . 2_565 ? 
OW2 Ca2 OW2 5.2(6) 6_565 2_565 ? 
OW2 Ca2 OW2 109.8(5) 2 2_565 ? 
OW2 Ca2 OW2 4.7(3) 5_565 2_565 ? 
OW2 Ca2 OW2 120.1(3) 6 2_565 ? 
OW2 Ca2 OW2 7.1(5) 1_565 2_565 ? 
Ca2 Ca2 OW2 57.4(3) 5_565 2_565 ? 
OW2 Ca2 OW2 114.5(5) 5 2_565 ? 
OW2 Ca2 O4 95.1(4) . . ? 
OW2 Ca2 O4 95.1(4) 6_565 . ? 
OW2 Ca2 O4 101.6(3) 2 . ? 
OW2 Ca2 O4 101.6(3) 5_565 . ? 
OW2 Ca2 O4 94.5(3) 6 . ? 
OW2 Ca2 O4 94.5(3) 1_565 . ? 
Ca2 Ca2 O4 105.0(2) 5_565 . ? 
OW2 Ca2 O4 100.3(3) 5 . ? 
OW2 Ca2 O4 100.3(3) 2_565 . ? 
OW2 Ca2 O1 89.8(4) . 5_565 ? 
OW2 Ca2 O1 89.8(4) 6_565 5_565 ? 
OW2 Ca2 O1 84.0(3) 2 5_565 ? 
OW2 Ca2 O1 84.0(3) 5_565 5_565 ? 
OW2 Ca2 O1 89.8(3) 6 5_565 ? 
OW2 Ca2 O1 89.8(3) 1_565 5_565 ? 
Ca2 Ca2 O1 84.37(18) 5_565 5_565 ? 
OW2 Ca2 O1 84.7(3) 5 5_565 ? 
OW2 Ca2 O1 84.7(3) 2_565 5_565 ? 
O4 Ca2 O1 170.62(18) . 5_565 ? 
OW2 Ca2 O2 167.1(3) . 1_565 ? 
OW2 Ca2 O2 76.3(3) 6_565 1_565 ? 
OW2 Ca2 O2 170.5(4) 2 1_565 ? 
OW2 Ca2 O2 81.7(3) 5_565 1_565 ? 
OW2 Ca2 O2 162.8(3) 6 1_565 ? 
OW2 Ca2 O2 72.1(3) 1_565 1_565 ? 
Ca2 Ca2 O2 134.39(7) 5_565 1_565 ? 
OW2 Ca2 O2 166.7(3) 5 1_565 ? 
OW2 Ca2 O2 77.1(2) 2_565 1_565 ? 
O4 Ca2 O2 83.23(11) . 1_565 ? 
O1 Ca2 O2 90.20(12) 5_565 1_565 ? 
OW2 Ca2 O2 76.3(3) . . ? 
OW2 Ca2 O2 167.1(3) 6_565 . ? 
OW2 Ca2 O2 81.7(3) 2 . ? 
OW2 Ca2 O2 170.5(4) 5_565 . ? 
OW2 Ca2 O2 72.1(3) 6 . ? 
OW2 Ca2 O2 162.8(3) 1_565 . ? 
Ca2 Ca2 O2 134.39(7) 5_565 . ? 
OW2 Ca2 O2 77.1(2) 5 . ? 
OW2 Ca2 O2 166.7(3) 2_565 . ? 
O4 Ca2 O2 83.23(11) . . ? 
O1 Ca2 O2 90.20(12) 5_565 . ? 
O2 Ca2 O2 90.72(14) 1_565 . ? 
OW2 Ca2 O1 67.9(4) . . ? 
OW2 Ca2 O1 67.9(4) 6_565 . ? 
OW2 Ca2 O1 68.9(3) 2 . ? 
OW2 Ca2 O1 68.9(3) 5_565 . ? 
OW2 Ca2 O1 70.7(3) 6 . ? 
OW2 Ca2 O1 70.7(3) 1_565 . ? 
Ca2 Ca2 O1 49.52(15) 5_565 . ? 
OW2 Ca2 O1 71.4(3) 5 . ? 
OW2 Ca2 O1 71.4(3) 2_565 . ? 
O4 Ca2 O1 55.49(10) . . ? 
O1 Ca2 O1 133.88(14) 5_565 . ? 
O2 Ca2 O1 120.26(11) 1_565 . ? 
O2 Ca2 O1 120.26(11) . . ? 
OW2 Ca2 V1 80.7(4) . . ? 
OW2 Ca2 V1 80.7(4) 6_565 . ? 
OW2 Ca2 V1 84.9(3) 2 . ? 
OW2 Ca2 V1 84.9(3) 5_565 . ? 
OW2 Ca2 V1 81.9(3) 6 . ? 
OW2 Ca2 V1 81.9(3) 1_565 . ? 
Ca2 Ca2 V1 77.38(17) 5_565 . ? 
OW2 Ca2 V1 85.5(3) 5 . ? 
OW2 Ca2 V1 85.5(3) 2_565 . ? 
O4 Ca2 V1 27.63(7) . . ? 
O1 Ca2 V1 161.75(15) 5_565 . ? 
O2 Ca2 V1 102.52(10) 1_565 . ? 
O2 Ca2 V1 102.52(10) . . ? 
O1 Ca2 V1 27.86(5) . . ? 
OW2 Ca2 Ca2 148.3(3) . 1_565 ? 
OW2 Ca2 Ca2 31.7(3) 6_565 1_565 ? 
OW2 Ca2 Ca2 142.6(3) 2 1_565 ? 
OW2 Ca2 Ca2 37.4(3) 5_565 1_565 ? 
OW2 Ca2 Ca2 152.6(3) 6 1_565 ? 
OW2 Ca2 Ca2 27.4(3) 1_565 1_565 ? 
Ca2 Ca2 Ca2 90.0 5_565 1_565 ? 
OW2 Ca2 Ca2 147.3(2) 5 1_565 ? 
OW2 Ca2 Ca2 32.7(2) 2_565 1_565 ? 
O4 Ca2 Ca2 90.0 . 1_565 ? 
O1 Ca2 Ca2 90.0 5_565 1_565 ? 
O2 Ca2 Ca2 44.64(7) 1_565 1_565 ? 
O2 Ca2 Ca2 135.36(7) . 1_565 ? 
O1 Ca2 Ca2 90.0 . 1_565 ? 
V1 Ca2 Ca2 90.0 . 1_565 ? 
OW2 Ca2 Ca2 31.7(3) . 1_545 ? 
OW2 Ca2 Ca2 148.3(3) 6_565 1_545 ? 
OW2 Ca2 Ca2 37.4(3) 2 1_545 ? 
OW2 Ca2 Ca2 142.6(3) 5_565 1_545 ? 
OW2 Ca2 Ca2 27.4(3) 6 1_545 ? 
OW2 Ca2 Ca2 152.6(3) 1_565 1_545 ? 
Ca2 Ca2 Ca2 90.0 5_565 1_545 ? 
OW2 Ca2 Ca2 32.7(2) 5 1_545 ? 
OW2 Ca2 Ca2 147.3(2) 2_565 1_545 ? 
O4 Ca2 Ca2 90.0 . 1_545 ? 
O1 Ca2 Ca2 90.0 5_565 1_545 ? 
O2 Ca2 Ca2 135.36(7) 1_565 1_545 ? 
O2 Ca2 Ca2 44.64(7) . 1_545 ? 
O1 Ca2 Ca2 90.0 . 1_545 ? 
V1 Ca2 Ca2 90.0 . 1_545 ? 
Ca2 Ca2 Ca2 180.0(2) 1_565 1_545 ? 
OW2 Ca2 V1 80.1(3) . 5_565 ? 
OW2 Ca2 V1 80.1(3) 6_565 5_565 ? 
OW2 Ca2 V1 73.1(3) 2 5_565 ? 
OW2 Ca2 V1 73.1(3) 5_565 5_565 ? 
OW2 Ca2 V1 81.3(3) 6 5_565 ? 
OW2 Ca2 V1 81.3(3) 1_565 5_565 ? 
Ca2 Ca2 V1 65.61(15) 5_565 5_565 ? 
OW2 Ca2 V1 75.0(3) 5 5_565 ? 
OW2 Ca2 V1 75.0(3) 2_565 5_565 ? 
O4 Ca2 V1 170.62(15) . 5_565 ? 
O1 Ca2 V1 18.76(7) 5_565 5_565 ? 
O2 Ca2 V1 103.25(10) 1_565 5_565 ? 
O2 Ca2 V1 103.25(10) . 5_565 ? 
O1 Ca2 V1 115.13(11) . 5_565 ? 
V1 Ca2 V1 142.99(11) . 5_565 ? 
Ca2 Ca2 V1 90.0 1_565 5_565 ? 
Ca2 Ca2 V1 90.0 1_545 5_565 ? 
OW2 Ca2 V2 148.8(3) . 1_565 ? 
OW2 Ca2 V2 91.6(3) 6_565 1_565 ? 
OW2 Ca2 V2 156.1(4) 2 1_565 ? 
OW2 Ca2 V2 98.2(3) 5_565 1_565 ? 
OW2 Ca2 V2 144.9(3) 6 1_565 ? 
OW2 Ca2 V2 87.5(3) 1_565 1_565 ? 
Ca2 Ca2 V2 149.24(7) 5_565 1_565 ? 
OW2 Ca2 V2 151.5(2) 5 1_565 ? 
OW2 Ca2 V2 93.5(2) 2_565 1_565 ? 
O4 Ca2 V2 67.87(8) . 1_565 ? 
O1 Ca2 V2 104.08(11) 5_565 1_565 ? 
O2 Ca2 V2 20.54(6) 1_565 1_565 ? 
O2 Ca2 V2 75.82(9) . 1_565 ? 
O1 Ca2 V2 115.88(9) . 1_565 ? 
V1 Ca2 V2 91.83(7) . 1_565 ? 
Ca2 Ca2 V2 60.93(3) 1_565 1_565 ? 
Ca2 Ca2 V2 119.07(3) 1_545 1_565 ? 
V1 Ca2 V2 120.02(8) 5_565 1_565 ? 
OW2 Ca2 V2 91.6(3) . . ? 
OW2 Ca2 V2 148.8(3) 6_565 . ? 
OW2 Ca2 V2 98.2(3) 2 . ? 
OW2 Ca2 V2 156.1(4) 5_565 . ? 
OW2 Ca2 V2 87.5(3) 6 . ? 
OW2 Ca2 V2 144.9(3) 1_565 . ? 
Ca2 Ca2 V2 149.24(7) 5_565 . ? 
OW2 Ca2 V2 93.5(2) 5 . ? 
OW2 Ca2 V2 151.5(2) 2_565 . ? 
O4 Ca2 V2 67.87(8) . . ? 
O1 Ca2 V2 104.08(11) 5_565 . ? 
O2 Ca2 V2 75.82(9) 1_565 . ? 
O2 Ca2 V2 20.54(6) . . ? 
O1 Ca2 V2 115.88(9) . . ? 
V1 Ca2 V2 91.83(7) . . ? 
Ca2 Ca2 V2 119.07(3) 1_565 . ? 
Ca2 Ca2 V2 60.93(3) 1_545 . ? 
V1 Ca2 V2 120.02(8) 5_565 . ? 
V2 Ca2 V2 58.14(6) 1_565 . ? 
O1 V1 O4 104.56(13) . . ? 
O1 V1 O7 104.40(8) . 1_565 ? 
O4 V1 O7 96.69(7) . 1_565 ? 
O1 V1 O7 104.40(8) . . ? 
O4 V1 O7 96.69(7) . . ? 
O7 V1 O7 143.89(14) 1_565 . ? 
O1 V1 O7 111.43(12) . 7 ? 
O4 V1 O7 144.01(11) . 7 ? 
O7 V1 O7 74.75(7) 1_565 7 ? 
O7 V1 O7 74.75(7) . 7 ? 
O1 V1 O3 169.28(10) . . ? 
O4 V1 O3 64.72(9) . . ? 
O7 V1 O3 77.88(7) 1_565 . ? 
O7 V1 O3 77.88(7) . . ? 
O7 V1 O3 79.29(9) 7 . ? 
O1 V1 V1 112.83(8) . 7_565 ? 
O4 V1 V1 126.35(6) . 7_565 ? 
O7 V1 V1 38.42(7) 1_565 7_565 ? 
O7 V1 V1 109.06(8) . 7_565 ? 
O7 V1 V1 36.32(2) 7 7_565 ? 
O3 V1 V1 75.60(5) . 7_565 ? 
O1 V1 V1 112.83(8) . 7 ? 
O4 V1 V1 126.35(6) . 7 ? 
O7 V1 V1 109.06(8) 1_565 7 ? 
O7 V1 V1 38.42(7) . 7 ? 
O7 V1 V1 36.32(2) 7 7 ? 
O3 V1 V1 75.60(5) . 7 ? 
V1 V1 V1 71.43(4) 7_565 7 ? 
O1 V1 V3 138.68(10) . . ? 
O4 V1 V3 34.12(8) . . ? 
O7 V1 V3 86.29(7) 1_565 . ? 
O7 V1 V3 86.29(7) . . ? 
O7 V1 V3 109.89(8) 7 . ? 
O3 V1 V3 30.60(5) . . ? 
V1 V1 V3 100.34(3) 7_565 . ? 
V1 V1 V3 100.34(3) 7 . ? 
O1 V1 Ca2 65.63(11) . . ? 
O4 V1 Ca2 38.93(9) . . ? 
O7 V1 Ca2 105.73(7) 1_565 . ? 
O7 V1 Ca2 105.73(7) . . ? 
O7 V1 Ca2 177.06(9) 7 . ? 
O3 V1 Ca2 103.65(8) . . ? 
V1 V1 Ca2 144.075(19) 7_565 . ? 
V1 V1 Ca2 144.075(19) 7 . ? 
V3 V1 Ca2 73.05(6) . . ? 
O1 V1 V1 90.0 . 1_565 ? 
O4 V1 V1 90.0 . 1_565 ? 
O7 V1 V1 18.06(7) 1_565 1_565 ? 
O7 V1 V1 161.94(7) . 1_565 ? 
O7 V1 V1 90.0 7 1_565 ? 
O3 V1 V1 90.0 . 1_565 ? 
V1 V1 V1 54.287(18) 7_565 1_565 ? 
V1 V1 V1 125.713(18) 7 1_565 ? 
V3 V1 V1 90.0 . 1_565 ? 
Ca2 V1 V1 90.0 . 1_565 ? 
O1 V1 V1 90.0 . 1_545 ? 
O4 V1 V1 90.0 . 1_545 ? 
O7 V1 V1 161.94(7) 1_565 1_545 ? 
O7 V1 V1 18.06(7) . 1_545 ? 
O7 V1 V1 90.0 7 1_545 ? 
O3 V1 V1 90.0 . 1_545 ? 
V1 V1 V1 125.713(18) 7_565 1_545 ? 
V1 V1 V1 54.287(18) 7 1_545 ? 
V3 V1 V1 90.0 . 1_545 ? 
Ca2 V1 V1 90.0 . 1_545 ? 
V1 V1 V1 180.00(4) 1_565 1_545 ? 
O1 V1 Ca2 28.62(11) . 5_565 ? 
O4 V1 Ca2 75.94(9) . 5_565 ? 
O7 V1 Ca2 107.87(7) 1_565 5_565 ? 
O7 V1 Ca2 107.87(7) . 5_565 ? 
O7 V1 Ca2 140.05(9) 7 5_565 ? 
O3 V1 Ca2 140.66(8) . 5_565 ? 
V1 V1 Ca2 133.02(4) 7_565 5_565 ? 
V1 V1 Ca2 133.02(4) 7 5_565 ? 
V3 V1 Ca2 110.06(6) . 5_565 ? 
Ca2 V1 Ca2 37.01(11) . 5_565 ? 
V1 V1 Ca2 90.0 1_565 5_565 ? 
V1 V1 Ca2 90.0 1_545 5_565 ? 
O2 V2 O5 102.47(12) . . ? 
O2 V2 O8 102.99(7) . . ? 
O5 V2 O8 98.35(7) . . ? 
O2 V2 O8 102.99(7) . 1_545 ? 
O5 V2 O8 98.35(7) . 1_545 ? 
O8 V2 O8 145.10(14) . 1_545 ? 
O2 V2 O6 99.68(12) . . ? 
O5 V2 O6 157.85(10) . . ? 
O8 V2 O6 76.50(7) . . ? 
O8 V2 O6 76.50(7) 1_545 . ? 
O2 V2 O8 178.36(11) . 7_655 ? 
O5 V2 O8 79.17(10) . 7_655 ? 
O8 V2 O8 76.68(7) . 7_655 ? 
O8 V2 O8 76.68(7) 1_545 7_655 ? 
O6 V2 O8 78.68(9) . 7_655 ? 
O2 V2 V3 136.64(10) . 7_655 ? 
O5 V2 V3 34.17(8) . 7_655 ? 
O8 V2 V3 88.44(7) . 7_655 ? 
O8 V2 V3 88.44(7) 1_545 7_655 ? 
O6 V2 V3 123.68(6) . 7_655 ? 
O8 V2 V3 45.00(6) 7_655 7_655 ? 
O2 V2 V3 98.36(8) . . ? 
O5 V2 V3 139.78(4) . . ? 
O8 V2 V3 43.08(7) . . ? 
O8 V2 V3 110.00(7) 1_545 . ? 
O6 V2 V3 34.203(16) . . ? 
O8 V2 V3 80.29(5) 7_655 . ? 
V3 V2 V3 116.95(2) 7_655 . ? 
O2 V2 V3 98.36(8) . 1_545 ? 
O5 V2 V3 139.78(4) . 1_545 ? 
O8 V2 V3 110.00(7) . 1_545 ? 
O8 V2 V3 43.08(7) 1_545 1_545 ? 
O6 V2 V3 34.203(16) . 1_545 ? 
O8 V2 V3 80.29(5) 7_655 1_545 ? 
V3 V2 V3 116.95(2) 7_655 1_545 ? 
V3 V2 V3 68.40(3) . 1_545 ? 
O2 V2 V2 146.12(3) . 7_655 ? 
O5 V2 V2 87.15(7) . 7_655 ? 
O8 V2 V2 43.15(7) . 7_655 ? 
O8 V2 V2 107.67(7) 1_545 7_655 ? 
O6 V2 V2 74.31(6) . 7_655 ? 
O8 V2 V2 33.53(2) 7_655 7_655 ? 
V3 V2 V2 59.17(2) 7_655 7_655 ? 
V3 V2 V2 57.78(3) . 7_655 ? 
V3 V2 V2 94.33(4) 1_545 7_655 ? 
O2 V2 V2 146.12(3) . 7_645 ? 
O5 V2 V2 87.15(7) . 7_645 ? 
O8 V2 V2 107.67(7) . 7_645 ? 
O8 V2 V2 43.15(7) 1_545 7_645 ? 
O6 V2 V2 74.31(6) . 7_645 ? 
O8 V2 V2 33.53(2) 7_655 7_645 ? 
V3 V2 V2 59.17(2) 7_655 7_645 ? 
V3 V2 V2 94.33(4) . 7_645 ? 
V3 V2 V2 57.78(3) 1_545 7_645 ? 
V2 V2 V2 65.57(3) 7_655 7_645 ? 
O2 V2 V2 90.0 . 1_545 ? 
O5 V2 V2 90.0 . 1_545 ? 
O8 V2 V2 162.55(7) . 1_545 ? 
O8 V2 V2 17.45(7) 1_545 1_545 ? 
O6 V2 V2 90.0 . 1_545 ? 
O8 V2 V2 90.0 7_655 1_545 ? 
V3 V2 V2 90.0 7_655 1_545 ? 
V3 V2 V2 124.200(16) . 1_545 ? 
V3 V2 V2 55.800(16) 1_545 1_545 ? 
V2 V2 V2 122.784(17) 7_655 1_545 ? 
V2 V2 V2 57.216(17) 7_645 1_545 ? 
O2 V2 V2 90.0 . 1_565 ? 
O5 V2 V2 90.0 . 1_565 ? 
O8 V2 V2 17.45(7) . 1_565 ? 
O8 V2 V2 162.55(7) 1_545 1_565 ? 
O6 V2 V2 90.0 . 1_565 ? 
O8 V2 V2 90.0 7_655 1_565 ? 
V3 V2 V2 90.0 7_655 1_565 ? 
V3 V2 V2 55.800(16) . 1_565 ? 
V3 V2 V2 124.200(16) 1_545 1_565 ? 
V2 V2 V2 57.216(17) 7_655 1_565 ? 
V2 V2 V2 122.784(17) 7_645 1_565 ? 
V2 V2 V2 180.000(18) 1_545 1_565 ? 
O2 V2 Ca2 33.60(6) . 1_545 ? 
O5 V2 Ca2 116.01(9) . 1_545 ? 
O8 V2 Ca2 126.74(8) . 1_545 ? 
O8 V2 Ca2 70.80(7) 1_545 1_545 ? 
O6 V2 Ca2 83.05(8) . 1_545 ? 
O8 V2 Ca2 145.59(5) 7_655 1_545 ? 
V3 V2 Ca2 141.95(5) 7_655 1_545 ? 
V3 V2 Ca2 100.28(6) . 1_545 ? 
V3 V2 Ca2 68.43(5) 1_545 1_545 ? 
V2 V2 Ca2 156.84(6) 7_655 1_545 ? 
V2 V2 Ca2 113.15(4) 7_645 1_545 ? 
V2 V2 Ca2 60.93(3) 1_545 1_545 ? 
V2 V2 Ca2 119.07(3) 1_565 1_545 ? 
O2 V2 Ca2 33.60(6) . . ? 
O5 V2 Ca2 116.01(9) . . ? 
O8 V2 Ca2 70.80(7) . . ? 
O8 V2 Ca2 126.74(8) 1_545 . ? 
O6 V2 Ca2 83.05(8) . . ? 
O8 V2 Ca2 145.59(5) 7_655 . ? 
V3 V2 Ca2 141.95(5) 7_655 . ? 
V3 V2 Ca2 68.43(5) . . ? 
V3 V2 Ca2 100.28(6) 1_545 . ? 
V2 V2 Ca2 113.15(4) 7_655 . ? 
V2 V2 Ca2 156.84(6) 7_645 . ? 
V2 V2 Ca2 119.07(3) 1_545 . ? 
V2 V2 Ca2 60.93(3) 1_565 . ? 
Ca2 V2 Ca2 58.14(6) 1_545 . ? 
O2 V2 Ca1 77.9(2) . . ? 
O5 V2 Ca1 24.6(2) . . ? 
O8 V2 Ca1 103.95(8) . . ? 
O8 V2 Ca1 103.95(8) 1_545 . ? 
O6 V2 Ca1 177.6(2) . . ? 
O8 V2 Ca1 103.7(2) 7_655 . ? 
V3 V2 Ca1 58.74(19) 7_655 . ? 
V3 V2 Ca1 145.750(19) . . ? 
V3 V2 Ca1 145.750(19) 1_545 . ? 
V2 V2 Ca1 107.69(16) 7_655 . ? 
V2 V2 Ca1 107.69(16) 7_645 . ? 
V2 V2 Ca1 90.0 1_545 . ? 
V2 V2 Ca1 90.000(1) 1_565 . ? 
Ca2 V2 Ca1 94.84(18) 1_545 . ? 
Ca2 V2 Ca1 94.84(18) . . ? 
O3 V3 O6 105.76(7) . 1_565 ? 
O3 V3 O6 105.76(7) . . ? 
O6 V3 O6 148.43(13) 1_565 . ? 
O3 V3 O4 96.56(12) . . ? 
O6 V3 O4 87.44(7) 1_565 . ? 
O6 V3 O4 87.44(7) . . ? 
O3 V3 O5 94.37(12) . 7_655 ? 
O6 V3 O5 89.60(7) 1_565 7_655 ? 
O6 V3 O5 89.60(7) . 7_655 ? 
O4 V3 O5 169.07(10) . 7_655 ? 
O3 V3 O8 171.97(11) . . ? 
O6 V3 O8 74.51(7) 1_565 . ? 
O6 V3 O8 74.51(7) . . ? 
O4 V3 O8 91.47(10) . . ? 
O5 V3 O8 77.60(9) 7_655 . ? 
O3 V3 V1 66.60(10) . . ? 
O6 V3 V1 95.47(7) 1_565 . ? 
O6 V3 V1 95.47(7) . . ? 
O4 V3 V1 29.96(7) . . ? 
O5 V3 V1 160.97(7) 7_655 . ? 
O8 V3 V1 121.43(7) . . ? 
O3 V3 V2 124.26(10) . 7_655 ? 
O6 V3 V2 81.86(6) 1_565 7_655 ? 
O6 V3 V2 81.86(6) . 7_655 ? 
O4 V3 V2 139.18(7) . 7_655 ? 
O5 V3 V2 29.89(7) 7_655 7_655 ? 
O8 V3 V2 47.71(6) . 7_655 ? 
V1 V3 V2 169.14(2) . 7_655 ? 
O3 V3 V2 145.786(16) . 1_565 ? 
O6 V3 V2 40.03(6) 1_565 1_565 ? 
O6 V3 V2 108.42(7) . 1_565 ? 
O4 V3 V2 83.73(6) . 1_565 ? 
O5 V3 V2 87.24(6) 7_655 1_565 ? 
O8 V3 V2 35.24(2) . 1_565 ? 
V1 V3 V2 108.35(3) . 1_565 ? 
V2 V3 V2 63.05(2) 7_655 1_565 ? 
O3 V3 V2 145.786(16) . . ? 
O6 V3 V2 108.42(7) 1_565 . ? 
O6 V3 V2 40.03(6) . . ? 
O4 V3 V2 83.73(6) . . ? 
O5 V3 V2 87.24(6) 7_655 . ? 
O8 V3 V2 35.24(2) . . ? 
V1 V3 V2 108.35(3) . . ? 
V2 V3 V2 63.05(2) 7_655 . ? 
V2 V3 V2 68.40(3) 1_565 . ? 
O3 V3 Ca1 53.8(4) . 7_655 ? 
O6 V3 Ca1 99.89(12) 1_565 7_655 ? 
O6 V3 Ca1 99.89(11) . 7_655 ? 
O4 V3 Ca1 150.3(4) . 7_655 ? 
O5 V3 Ca1 40.6(4) 7_655 7_655 ? 
O8 V3 Ca1 118.2(4) . 7_655 ? 
V1 V3 Ca1 120.4(4) . 7_655 ? 
V2 V3 Ca1 70.5(4) 7_655 7_655 ? 
V2 V3 Ca1 120.1(3) 1_565 7_655 ? 
V2 V3 Ca1 120.1(3) . 7_655 ? 
O3 V3 V3 90.0 . 1_565 ? 
O6 V3 V3 15.78(7) 1_565 1_565 ? 
O6 V3 V3 164.22(7) . 1_565 ? 
O4 V3 V3 90.0 . 1_565 ? 
O5 V3 V3 90.0 7_655 1_565 ? 
O8 V3 V3 90.0 . 1_565 ? 
V1 V3 V3 90.0 . 1_565 ? 
V2 V3 V3 90.0 7_655 1_565 ? 
V2 V3 V3 55.800(16) 1_565 1_565 ? 
V2 V3 V3 124.200(16) . 1_565 ? 
Ca1 V3 V3 90.000(1) 7_655 1_565 ? 
O3 V3 V3 90.0 . 1_545 ? 
O6 V3 V3 164.22(7) 1_565 1_545 ? 
O6 V3 V3 15.78(7) . 1_545 ? 
O4 V3 V3 90.0 . 1_545 ? 
O5 V3 V3 90.0 7_655 1_545 ? 
O8 V3 V3 90.0 . 1_545 ? 
V1 V3 V3 90.0 . 1_545 ? 
V2 V3 V3 90.0 7_655 1_545 ? 
V2 V3 V3 124.200(16) 1_565 1_545 ? 
V2 V3 V3 55.800(16) . 1_545 ? 
Ca1 V3 V3 90.000(1) 7_655 1_545 ? 
V3 V3 V3 180.00(4) 1_565 1_545 ? 
O3 V3 Ca1 56.7(4) . 3 ? 
O6 V3 Ca1 99.24(11) 1_565 3 ? 
O6 V3 Ca1 99.24(11) . 3 ? 
O4 V3 Ca1 153.3(4) . 3 ? 
O5 V3 Ca1 37.6(4) 7_655 3 ? 
O8 V3 Ca1 115.2(4) . 3 ? 
V1 V3 Ca1 123.3(4) . 3 ? 
V2 V3 Ca1 67.5(4) 7_655 3 ? 
V2 V3 Ca1 117.8(3) 1_565 3 ? 
V2 V3 Ca1 117.8(3) . 3 ? 
Ca1 V3 Ca1 3.0(8) 7_655 3 ? 
V3 V3 Ca1 90.000(1) 1_565 3 ? 
V3 V3 Ca1 90.0 1_545 3 ? 
O3 V3 Ca2 123.70(11) . . ? 
O6 V3 Ca2 80.67(7) 1_565 . ? 
O6 V3 Ca2 80.67(7) . . ? 
O4 V3 Ca2 27.14(8) . . ? 
O5 V3 Ca2 141.93(9) 7_655 . ? 
O8 V3 Ca2 64.33(8) . . ? 
V1 V3 Ca2 57.10(5) . . ? 
V2 V3 Ca2 112.04(6) 7_655 . ? 
V2 V3 Ca2 61.89(5) 1_565 . ? 
V2 V3 Ca2 61.89(5) . . ? 
Ca1 V3 Ca2 177.4(4) 7_655 . ? 
V3 V3 Ca2 90.0 1_565 . ? 
V3 V3 Ca2 90.0 1_545 . ? 
Ca1 V3 Ca2 179.6(4) 3 . ? 
V1 O1 Ca2 132.62(16) . 5_565 ? 
V1 O1 Ca2 86.50(12) . . ? 
Ca2 O1 Ca2 46.12(14) 5_565 . ? 
V2 O2 Ca2 125.86(10) . 1_545 ? 
V2 O2 Ca2 125.86(10) . . ? 
Ca2 O2 Ca2 90.72(14) 1_545 . ? 
V3 O3 Ca1 99.3(6) . 7_655 ? 
V3 O3 V1 82.81(11) . . ? 
Ca1 O3 V1 177.9(6) 7_655 . ? 
V3 O3 Ca1 98.2(5) . 3 ? 
Ca1 O3 Ca1 1.1(11) 7_655 3 ? 
V1 O3 Ca1 179.0(5) . 3 ? 
V1 O4 V3 115.92(13) . . ? 
V1 O4 Ca2 113.44(14) . . ? 
V3 O4 Ca2 130.64(14) . . ? 
V2 O5 V3 115.94(13) . 7_655 ? 
V2 O5 Ca1 137.5(4) . . ? 
V3 O5 Ca1 106.5(4) 7_655 . ? 
V2 O5 Ca1 130.6(4) . 5_655 ? 
V3 O5 Ca1 113.4(4) 7_655 5_655 ? 
Ca1 O5 Ca1 6.9(8) . 5_655 ? 
V3 O6 V3 148.43(13) . 1_545 ? 
V3 O6 V2 105.77(7) . . ? 
V3 O6 V2 105.77(7) 1_545 . ? 
V1 O7 V1 143.89(14) 1_545 . ? 
V1 O7 V1 105.25(7) 1_545 7 ? 
V1 O7 V1 105.25(7) . 7 ? 
V2 O8 V2 145.10(14) . 1_565 ? 
V2 O8 V3 101.69(7) . . ? 
V2 O8 V3 101.69(7) 1_565 . ? 
V2 O8 V2 103.32(7) . 7_655 ? 
V2 O8 V2 103.32(7) 1_565 7_655 ? 
V3 O8 V2 87.30(9) . 7_655 ? 
Ca1 OW1 Ca1 105.3(9) . 1_565 ? 
Ca1 OW1 Ca1 6.7(6) . 5_655 ? 
Ca1 OW1 Ca1 100.89(13) 1_565 5_655 ? 
Ca1 OW1 Ca1 100.89(13) . 5_665 ? 
Ca1 OW1 Ca1 6.7(6) 1_565 5_665 ? 
Ca1 OW1 Ca1 96.0(7) 5_655 5_665 ? 
OW2 OW2 OW2 90.00(3) 2 6 ? 
OW2 OW2 OW2 46(2) 2 5 ? 
OW2 OW2 OW2 44(2) 6 5 ? 
OW2 OW2 Ca2 112.7(19) 2 . ? 
OW2 OW2 Ca2 148.3(3) 6 . ? 
OW2 OW2 Ca2 151(3) 5 . ? 
OW2 OW2 Ca2 59.4(17) 2 5_565 ? 
OW2 OW2 Ca2 142.6(4) 6 5_565 ? 
OW2 OW2 Ca2 102(2) 5 5_565 ? 
Ca2 OW2 Ca2 68.9(4) . 5_565 ? 
OW2 OW2 Ca2 109.8(16) 2 1_545 ? 
OW2 OW2 Ca2 27.4(3) 6 1_545 ? 
OW2 OW2 Ca2 67(2) 5 1_545 ? 
Ca2 OW2 Ca2 120.9(6) . 1_545 ? 
Ca2 OW2 Ca2 168.8(6) 5_565 1_545 ? 
OW2 OW2 Ca2 63.1(15) 2 5 ? 
OW2 OW2 Ca2 32.7(2) 6 5 ? 
OW2 OW2 Ca2 23(3) 5 5 ? 
Ca2 OW2 Ca2 174.8(6) . 5 ? 
Ca2 OW2 Ca2 109.8(5) 5_565 5 ? 
Ca2 OW2 Ca2 59.9(3) 1_545 5 ? 
 
_diffrn_measured_fraction_theta_max    1.000 
_diffrn_reflns_theta_full              30.10 
_diffrn_measured_fraction_theta_full   1.000 
_refine_diff_density_max    0.619 
_refine_diff_density_min   -0.411 
_refine_diff_density_rms    0.116 
